4.2 Silicon compounds
4.2.2 Organic silicon compounds
In contrast to the inorganic silicon compounds discussed in the previous chapter, organic silicon compounds can be altered in their properties by different organic groups attached to the silicon (Mai and Militz, 2004a). Methyl groups can impart high hydrophobicity to the material combined with high thermal stability, while other groups might act biocidal or affect the orientation of the molecules after application to wood.
The sol-gel process mentioned above, which applies tetraalkoxysilanes can be varied by taking organosilanes as precursors. These molecules contain up to three silicon functional alkoxy groups and one to three organo-functional groups, which can increase hydrophobicity of the gel or form covalent bonds to other constituents.
Organo-silanes are used in many applications such as adhesion promotion, cross linking or surface modification (Mai and Militz, 2004a).
Schneider and Brebner (1985) used the coupling agent γ-methacryloxypropyltrimethoxysilane to treat different wood species in a sol-gel process and found ASE values of up to 70%. Donath et al. (2004) used, besides the before mentioned TEOS, also organo functional alkoxysilanes and found good incorporation into the cell wall, when conditioned wood was impregnated with alcoholic solutions of the two silanes methyltriethoxysilane and
15 propyltriethoxysilane. ASE values of up to 30% were measured, but this value decreased over time due to ageing of the gel in the cell wall. Durability of the treated wood towards the white rot fungus Trametes versicolor was increased considerably but especially, when the silane penetrated and bulked the cell wall. In a soil block test, decay was delayed, but not prevented. Further trials with the two alkylalkoxysilanes and two additional, oligomeric and water-borne silane systems revealed strong hydrophobation of the treated wood. This was more pronounced for the two oligomeric silane systems, and in addition the hydrophobation remained after several wetting and drying cycles, while it was reduced for the two alkylalkoxysilanes (Donath et al., 2006b).
Hill et al. (2004) treated pine sapwood (Pinus nigra) with the two coupling agents γ-methacryloxypropyltrimethoxysilane and vinyltrimethoxysilane. They found incorporation of the silicon material into the cell wall and ASE values of up to 40%. Fungal decay tests revealed only little increase of resistance to the brown rot fungus Coniophora puteana. Incubation with the white rot fungi Trametes versicolor and Phanerochaete crysosporium displayed decay resistance of the treated wood above a WPG of approx. 40% for Trametes versicolor and approx. 40-50% for Phanerochaete crysosporium (Hill et al., 2004).
Higher decay resistance was found, if amino-functional silanes were applied.
Donath et al. (2006a) treated wood with an amino-functional oligomeric silane system and found complete decay resistance of pine sapwood (Pinus sylvestris L.) to the brown rot fungus Coniophora puteana with a WPG of 16% even after prolonged incubation of 18 weeks. Beech wood (Fagus sylvatica L.) treated with the same silane and showing a WPG of 11%, however, showed considerable mass loss after incubation with Trametes versicolor (Donath et al., 2006a). Weathering of pine wood (Pinus sylvestris L.) revealed, that the water repellent effect of three monomeric alkylalkoxysilanes and two oligomeric silane systems remained stable over one year.
Sorption, however, was not affected and checking of the weathered samples not reduced as compared to control specimens (Donath et al., 2007).
Nami Kartal et al. (2009) treated wood with two different alkyl-alkoxy-functional silanes in combination with boric acid to limit boron leaching from the treated wood. They were able to reduce boron leaching by approx. 40% through this combination. The treated wood showed increased resistance to fungal and termite decay compared to wood treated solely with silane or boron.
While all studies mentioned above aimed on simply depositing the silicon material in the wood, a different approach is the covalent bonding of the silicon material to the wood. Sèbe et al. (2004) treated wood with different
organo-16 functional alkoxysilanes and were able to graft the silicon compounds to the hydroxyl groups of wood via carbamoylation and etherification by use of the organo-functionality and also by alcoholysis, which results in a direct reaction of the silanol with hydroxyl groups of the cell wall. The reactions were confirmed by WPG, infrared spectroscopy (FTIR) and 13C and 29Si NMR CP-MAS analysis. The treatment, however, resulted only in small ASE values, which decreased in a subsequent water soaking test (Sèbe et al., 2004). Further work on the carbamoylation of wood using isocyanatopropyltriethoxysilane was done by Tingaut et al. (2005; 2006).
Besides alkoxy silanes, chlorosilanes are a group of very reactive silicon compounds. Hydrophobation of organic material (paper) by methylchlorosilanes was first observed by W. Patnode in 1940 while producing methyl-chlorosilanes in a lab.
Evaporating silane hydrolyzed upon contact with the moisture in the air and reacted on and with the paper present in the lab (Rochow, 1991). This observation led to the idea of hydrophobizing materials with chlorosilanes (Patnode, 1942). During hydrolyzation of chlorosilanes, HCl is released, which is the major drawback of this idea, because wood, being sensitive to acid breakdown, will be degraded. Still some work was performed to treat wood with different chlorosilanes. Owens et al. (1980) treated wood with tetrachlorosilane and found increased decay resistance of the treated wood to brown and white rot fungi. Stevens (1981) used tetrachlorosilane, methyltrichlorosilane, dimethyldichlorosilane, methyldichloro-hydrogensilane and chlorotrimethylsilane to treat pine and beech wood in vapor and liquid phase. To avoid the degradation of wood by HCl, besides hexane different basic hydrochloric acid acceptors were used as solvents (triethylamine, formamide, dimethylformamide). This time the treatments, however, did not result in high decay resistance of pine sapwood (Pinus sylvestris L.) to Poria placenta and Gloeophyllum trabeum as well as beech wood (Fagus sylvatica L.) to Trametes versicolor and Coniophora puteana. Best results (weight losses of 5-10%) were obtained with the two materials dimethyldichlorosilane and methyldichlorohydrogensilane. Further examination of the effect on blue stains and moulds revealed only low effects of chlorosilane treatment (Stevens, 1985).
Another group of organo-silicon compounds are the silicones. These are polymeric materials with a silicon-oxygen backbone and hydrocarbon radicals attached directly to the silicon (Noll, 1968). The name silicone derives from the term silicon ketone, because the empirical formula (R2SiO)n is similar to the ketones from organic chemistry (R2CO) (Noll, 1968). The basic repeating unit in silicones is the siloxane, while the most common silicones are polydimethylsiloxanes (Figure 4).
17 Depending on the chain length and attached functionalities, PDMS are a class of polymers ranging from fluids to elastomers.
Figure 4: Unfunctional polydimethylsiloxane.
The synthesis of silicones uses methyl-chlorosilanes as precursors, which are prepared from elemental silicon by a direct synthesis found by Rochow and Müller simultaneously in 1940 (Schliebs and Ackermann, 1987) and which was the starting point for mass production of silicones:
2 CH3 Cl + Si [Cu]
These chlorosilanes are further hydrolyzed under formation of HCl and the resulting silanol groups subsequently polymerize to form polydimethylsiloxane (Ackermann and Damrath, 1989). Silicones are the only important polymer with an inorganic backbone, are physiological inert and hard to inflame. The methyl groups attached to the silicon have proved to be superior over other organic groups due to their small size and absence of carbon-carbon bonds which render the silicone very stable towards heat and chemicals (Rochow, 1991). That is the reason, why polydimethylsiloxane has become the most common silicone.
Recently, functionalized PDMS have attracted interest. Introduction of functional groups into the silicone structure offers the possibility to alter the properties of the silicone in specific ways, for example combine hydrophobic and hydrophilic properties. Examples for functional groups are esters, epoxides, vinyl-, allyl-, amino- and carboxy groups. Functionalized siloxanes have especially proved valuable for the combination of natural materials such as textiles and wood with PDMS. While unfunctional silicones do not interact with surfaces of textiles and wood, amino groups have proved to increase binding and orientation of PDMS on textile surfaces (Bereck et al., 2001). Due to the extreme flexibility of the siloxane backbone and the low surface energy, PDMS can spread on the surface of fibrous substrates and reduce friction of the fibers and increase hydrophobicity (Kim, 2001).
Bereck et al. (1996) studied the application of amino silicones on cotton and cotton-polyester textiles. The strongest influence on the properties of the treated
18 textiles was found in the amino group content of the siloxane. The position of amino groups on the siloxane backbone was also found to have a significant effect.
Softening of textiles was better for siloxane with aminogroups attached to the sides of the backbones compared to α-ω functional amino silicones, while the material also became more hydrophobic.
Kim (2001) studied hydrophobation of textiles with siloxane and found amino siloxanes very effective. A strong influence on hydrophobation was found for functionality, amino content, attachement of functional group and application of siloxane. Heating of the treated textile material after application of siloxane increased orientation of the PDMS (with hydrophilic parts facing the textile) and significantly enhanced hydrophobation.
While silicone treatment of masonry to improve water repellence without reduction of water vapor permeability and to increase service life is common, treatment of wood has not gained such an importance (Hager, 1995). Rochow, who is one of the inventors of the direct synthesis of methylchlorosilanes has laid the foundation for mass production of silicones He treated his wooden house in 1958 with a coating of silicones and even 30 years later found little degradation of the coating (Rochow, 1991). This shows the potential of silicone application for the protection of wooden constructions.
To avoid the use of organic solvents, water-borne formulations are preferred for treatment of wood. SMK micro emulsions (Wacker SMK® technology) were used by Hager (1995) to impregnate wood. The technology combines silanes, siloxanes and functional polysiloxanes, which are at the same time temporary emulsifiers and co-emulsifiers. After drying the emulsifiers lose their ability and serve as adhesion promoters and catalysts. Upon mixing with water, the system emulsifies itself and forms droplets of 10-80nm diameter, which are able to penetrate the wood structure and deposit the silicone in the lumens of the cells. Hager (1995) found a 70%
reduction of water uptake even after two years of outside weathering (10% silicone treatment), showing the long term effectiveness of the silicone. Lukowsky et al.
(1997) further investigated SMK type formulations of silicones and found high water repellence with long lasting stability. ASE, however, was not found and gluing of the specimens with PVAc revealed strong reduction of glue bond strength. Although the results are promising, the SMK technology has the major drawback of a short pot life of <24h, which is not applicable for the use in impregnation plants. Furthermore methanol and ethanol are split off and cause further problems in the treatment and drying processes.
19 Simon et al. (2011) treated wood with solvent based solutions of silicones and found strongly reduced water uptake of the treated wood. The concentrations (and WPG) that were used, however, were very high (up to 90%) and therefore not viable in practice. De Vetter et al. (2010) treated wood with different water-borne emulsions of silicones and found no significantly improved water repellence and no ASE for low WPG of approx. 5-6%. They concluded that only functionalized silicones may be effective enough for the treatment of wood.
The development of functional silicones, which have proved to be superior to unfunctional silicones in textiles, in combination with the similarities of the substrates cotton (textiles) and cellulose (wood) have led to the idea of using functional silicones to improve properties of wood. Weigenand et al (2007) studied the impregnation of wood with two amino-functional silicones formulated as micro- and macroemulsion, respectively. They found good penetration of the emulsions into the wood and also into the cell wall resulting in positive bulking values. These were higher for the micro- compared to the macroemulsion and resulted in positive ASE values. The cell wall penetration was further confirmed by x-ray mapping (SEM-EDX). Water repellence was especially high in the initial phase of water uptake, later on water repellent effectiveness (WRE) decreased.
The amino-silicone microemulsion was further investigated for its ability to impart decay resistance to the treated wood (Weigenand et al., 2008). Pine sapwood (Pinus sylvestris L.) and beech wood (Fagus sylvatica L.) was treated with 2, 5 and 15% concentrations of the amino-silicone and incubated with the brown rot fungi Coniophora puteana, Antrodia vaillantii, Gloeophyllum trabeum and Serpula lacrymans as well as the white rot fungi Trametes versicolor and Ceriporiopsis subvermispora and the soft rot fungus Hypoxylon fragiforme.
Decay in a test according to EN 113 was strongly reduced by the treatments for all fungi but the soft rot, when the wood had been treated with 15% emulsions. The resistance was mainly explained with the amino groups attached to the silicone (Weigenand et al., 2008).
The influence of silicone functionality on fungal decay of the treated wood was further evaluated by Ghosh et al. (2008). They treated pine sapwood (Pinus sylvestris L.) and beech wood (Fagus sylvatica L.) with three emulsions of commercially available silicones bearing different functionalities: alkyl-functional, amino-functional and quaternary-ammonium-amino-functional. While the alkyl-amino-functional silicone did not impart any resistance to wood in a mini block test according to Bravery (1978), the two other silicones considerably reduced mass loss due to incubation with Coniophora puteana (pine) and Trametes versicolor (beech) if high treatment
20 concentrations of 15% were used. In an unsterile soil bed test according to EN 807 silicone treated wood showed slightly reduced mass loss and loss of MOE compared to untreated wood. In both tests, amino-silicone showed somewhat better results than quarternary-ammonium-silicone (Ghosh et al., 2008).
The same silicone emulsions were tested on their ability to impart resistance to blue stain and mold fungi. While even treatment with 10% emulsions of alkyl- and quarternary-ammonium-functional silicone did not inhibit colonization by blue stain, amino-functional silicone did radically reduce infestation even with a concentration of 4%. Treatment with 10% amino-silicone also resulted in a certain resistance to mold growth, while the other two silicones showed lower effectiveness (Ghosh et al., 2009).
Further work revealed high effectiveness of the three silicone emulsions to termite attack. A field test with the two termite species Coptotermes acinaciformis (Froggatt) and Mastotermes darwiniensis (Froggatt) resulted in complete protection, when the pine sapwood had been treated with 5% emulsions of amino- and quarternary-ammonium-functional silicone. Alkyl-functional silicone treatment reduced mass loss, but was slightly less effective (Ghosh et al., 2012b).
As quarternary-ammonium- and amino-functional silicones showed promising results, further trials focused on these materials using different chain length. The silicones were solved in a mixture of water and organic solvents to avoid influence of the emulsifiers. Positive bulking and increased dimensional stability was found for pine sapwood; 30% treatment with amino-silicone with a chain length of 9 resulted in an ASE of approx. 60%. Pine sapwood and beech wood showed greatly reduced mass loss after 12 weeks of incubation with Coniophora puteana (pine) and Trametes versicolor (beech). Treatment with 15% short-chained quarternary-ammonium- and amino-functional silicone resulted in mass losses of less than 5% for pine sapwood. Increasing effectiveness against decay was found for decreasing chain length of the particular silicone (Ghosh, 2009).